General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.85 g/cm³ Show Material materials with Density of 7.85 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa | |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | ||

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | ||

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | ||

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | ||

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | ||

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | ||

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | ||

Elongation | 20.0 °C | 24 % Show Material materials with Elongation of 24 % | |

Poisson's ratio | 23.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | Typical for Nickel Steel |

Shear modulus | 23.0 °C | 76 GPa Show Material materials with Shear modulus of 76 GPa | Typical for Nickel Steel |

Tensile strength | 20.0 °C | 410 - 530 MPa Show Material materials with Tensile strength of 410 - 530 MPa | |

Yield strength | 20.0 °C | 265 - 285 MPa Show Material materials with Yield strength of 265 - 285 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.05E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 1/K | |

20.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | ||

100.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | ||

200.0 °C | 1.27E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.27E-5 1/K | ||

300.0 °C | 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 1/K | ||

400.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | ||

500.0 °C | 1.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.4E-5 1/K | ||

600.0 °C | 1.44E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.44E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1316 - 1595 °C Show Material materials with Melting point of 1316 - 1595 °C | Typical for Nickel Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 42.5 W/(m·K) Show Material materials with Thermal conductivity of 42.5 W/(m·K) | |

100.0 °C | 43.5 W/(m·K) Show Material materials with Thermal conductivity of 43.5 W/(m·K) | ||

200.0 °C | 42.8 W/(m·K) Show Material materials with Thermal conductivity of 42.8 W/(m·K) | ||

300.0 °C | 40.9 W/(m·K) Show Material materials with Thermal conductivity of 40.9 W/(m·K) | ||

400.0 °C | 39 W/(m·K) Show Material materials with Thermal conductivity of 39 W/(m·K) | ||

500.0 °C | 36.4 W/(m·K) Show Material materials with Thermal conductivity of 36.4 W/(m·K) | ||

600.0 °C | 34.1 W/(m·K) Show Material materials with Thermal conductivity of 34.1 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 11.7 mm²/s Show Material materials with Thermal diffusivity of 11.7 mm²/s | |

100.0 °C | 11.2 mm²/s Show Material materials with Thermal diffusivity of 11.2 mm²/s | ||

200.0 °C | 10.3 mm²/s Show Material materials with Thermal diffusivity of 10.3 mm²/s | ||

300.0 °C | 9.3 mm²/s Show Material materials with Thermal diffusivity of 9.3 mm²/s | ||

400.0 °C | 8.3 mm²/s Show Material materials with Thermal diffusivity of 8.3 mm²/s | ||

500.0 °C | 7 mm²/s Show Material materials with Thermal diffusivity of 7 mm²/s | ||

600.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 2.45E-7 Ω·m Show Material materials with Electrical resistivity of 2.45E-7 Ω·m |

100.0 °C | 2.94E-7 Ω·m Show Material materials with Electrical resistivity of 2.94E-7 Ω·m | |

200.0 °C | 3.69E-7 Ω·m Show Material materials with Electrical resistivity of 3.69E-7 Ω·m | |

300.0 °C | 4.59E-7 Ω·m Show Material materials with Electrical resistivity of 4.59E-7 Ω·m | |

400.0 °C | 5.58E-7 Ω·m Show Material materials with Electrical resistivity of 5.58E-7 Ω·m | |

500.0 °C | 6.79E-7 Ω·m Show Material materials with Electrical resistivity of 6.79E-7 Ω·m | |

600.0 °C | 8.13E-7 Ω·m Show Material materials with Electrical resistivity of 8.13E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.02 % Show Material materials with Aluminium of 0.02 % |

Carbon | 0.14 % Show Material materials with Carbon of 0.14 % |

Manganese | 0.7 - 1.5 % Show Material materials with Manganese of 0.7 - 1.5 % |

Nickel | 0.3 - 0.8 % Show Material materials with Nickel of 0.3 - 0.8 % |

Niobium | 0.05 % Show Material materials with Niobium of 0.05 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % |

Sulfur | 0.025 % Show Material materials with Sulfur of 0.025 % |

Vanadium | 0.05 % Show Material materials with Vanadium of 0.05 % |